2 Part 1 Phase Transformations in Metals Development of Microstructure and Alteration of Mechanical Properties
3 Why Study Phase Transformations in Metals? The development of a set of desirable mechanical properties for a material often results from a phase transformation, which is wrought by a heat treatment.The time and temperature dependencies of some phase transformations are conveniently represented on modified phase diagrams.It is important to know how to use these diagrams in order to design a heat treatment for some alloy that will yield the desired room-temperature mechanical properties.The tensile strength of an iron-carbon alloy of eutectoid composition (0.76wt% C) can be varied between ~ 700 MPa and 2000 MPa depending on the heat treatment employed.
4 How to tailor mechanical properties of metallic materials? Four strengthening mechanisms:Grain size refinementSolid-solution strengtheningStrain hardeningPrecipitation hardeningAdditional techniques are available wherein the mechanical properties are reliant on the characteristics of the microstructure.The development of microstructure in both single- and two-phase alloys ordinarily involves some type of phase transformation — an alteration in the number and/or character of the phases.
5 The iron–iron carbide phase diagram L + Fe3C2.144.306.700.0220.76MNCPEOGFHCementite Fe3Cxx’yy’zz’The iron–iron carbide phase diagram
7 Important Phases in the Iron-Iron Carbide System Thermal processing or heat treating: the art and science of controlling thermal energy for the purpose of altering the properties of metals and alloysFerrite (a-Fe): Pure Fe (room temperature to 912C), a single-phase BCC solid solutionFerrite can accommodate 0.022% carbon at 727C.Austenite (g-Fe): a single-phase FCC solid solutiona ferrite transforms from BCC to FCC at 912C.Characteristics: ability to be deformed and to absorb carbon up to 2.14% at 1147CCementite (iron carbide Fe3C): intermediate phase with the chemical formula Fe3C6.70% C: brittle and hard
8 The Iron–Iron Carbide Phase Diagram. L + Fe3C2.144.306.70MNCPEOGFHCementite Fe3Cxx’0.0220.76
9 Important Phases in the Iron-Iron Carbide System (Cont’d) Pearlite:When steel with the eutectoid composition forms at 727C, it produces a lamellar two- phase mixture of ferrite and cementiteHypoeutectoid steel: a mixture of ferrite and pearliteHypereutectoid steel: a mixture of pearlite and cementite
10 Pearlite Microstructure a ferrite(light phase)Fe3C(dark phase)Pearlite has mechanical properties between the soft, ductile ferrite and the hard, brittle cementite.Photomicrograph of a eutectoid steel showing the pearlite microstructure consisting of alternating layers of a ferrite (the light phase) and Fe3C (thin layers most of which appear dark). 500X.
11 The Iron-Iron Carbide System One eutectic reaction exists for the iron-iron carbide system, at 4.30wt% C and 1147C (Line PEG).L (4.30wt% C) g (2.14wt% C) + Fe3C (6.70wt% C)One eutectoid reaction exists for the iron-iron carbide system, at 0.76wt% C and 727C (Line NOH).g (0.76wt% C) a (0.022wt% C) + Fe3C (6.70wt% C)
12 Phase Transformations Phase Transformation: a change in the number and/or character of the phases that constitute the microstructure of an alloyIn general, two processes accompany the phase transformation such as the eutectoid reaction:Nucleation the formation of very small particles, or nuclei, of the new phaseFavorable nucleation sites: imperfection sites, especially grain boundariesGrowth the increase of the nuclei in sizeSome volume of the parent phase disappears.
13 The Iron–Iron Carbide Phase Diagram. L + Fe3C2.144.306.70MNCPEOGFHCementite Fe3Cxx’0.0220.76
14 The Limitation of Equilibrium Phase Diagrams Unable to indicate the time period required for the attainment of equilibriumEquilibrium conditions are maintained only if heating or cooling is carried out at extremely slow and unpractical rates.
15 Time-Temperature-Transformation (T-T-T) Diagrams PearliteThe eutectoid reaction is fundamental to the development of microstructures in steel alloys.g (0.76 wt% C) ⇌ a (0.022 wt% C) + Fe3C (6.70 wt% C)Pearlite is the microstructural product of this transformation.Interpretation of the TTT diagramAbove eutectoid temperature: only austenite existsBelow eutectoid temperature: nucleation + growthThe percentage of the transformation product is related to the holding temperature and holding time.
16 2.14 4.30 6.70 M N C P E O G F H Cementite Fe3C x x’ L + Fe3C2.144.306.70MNCPEOGFHCementite Fe3Cxx’0.0220.76The iron–iron carbide phase diagram
17 A: austenite B: bainite M: martensite P: pearlite The complete TTT diagram for an iron-carbon alloy of eutectoid composition.A: austeniteB: bainiteM: martensiteP: pearlite
19 Time-Temperature-Transformation (T-T-T) Diagrams PearliteThe thickness of the ferrite/cementite layers in pearlite depends on the temperature. With decreasing temperature, the layers become progressively thinner.At temperatures just below eutectoid relatively thick layers coarse pearliteIn the vicinity of 540C relatively thin layers fine pearlite
20 Photomicrographs of (a) coarse pearlite and (b) fine pearlite. 3000X.
21 A: austenite B: bainite M: martensite P: pearlite The complete isothermal transformation diagram for an iron-carbon alloy of eutectoid composition.A: austeniteB: bainiteM: martensiteP: pearlite
22 MartensiteMartensite is formed when austenitized Fe-C alloys are rapidly cooled (or quenched) to a relatively low temperature (in the vicinity of the ambient).Non-equilibrium single phaseA transformation product that is competitive with pearliteTransformation of FCC to BCT (body-centered tetragonal)Occurs instantaneously time-independentThe martensite grains nucleate and grow at a very rapid rate — the velocity of sound within the austenite matrix.
23 (body-centered tetragonal) FCC Austenite(g phase)BCT Martensite(body-centered tetragonal)The body-centered tetragonal unit cell for martensitic steel showing iron atoms (circles) and sites that may be occupied by carbon atoms (crosses). For this tetragonal unit cell, c > a.
24 Lenticular or plate martensitic microstructure Photomicrograph showing the lenticular or plate martensitic microstructure. The needle-shaped grains are the martensite phase, and the white regions are austenite that failed to transform during the rapid quench. 1220X.
25 A: austenite B: bainite M: martensite P: pearlite The complete isothermal transformation diagram for an iron-carbon alloy of eutectoid composition.A: austeniteB: bainiteM: martensiteP: pearlite
26 The Martensitic Transformation Since the martensitic transformation is instantaneous, it is not depicted in this diagram like the pearlitic reaction.The beginning of this transformation is represented by a horizontal line designated M(start).Two other horizontal and dashed lines, labeled M(50%) and M(90%), indicate percentages of the austenite-to-martensite transformation.The temperatures at which these lines are located vary with alloy composition; the temperatures must be relatively low.The horizontal and linear character of these lines indicates that the martensitic transformation is independent of time; it is a function only of the temperature to which the alloy is quenched.
27 Effects of alloying elements The presence of alloying elements other than carbon (e.g., Cr, Ni, Mo, and W) may cause significant changes in the positions/shapes of the curves in the isothermal transformation diagrams.TTT diagram for an alloy steel (type 4340):A, austenite;B, bainite;P, pearlite;M, martensite;F, proeuctectoid ferrite.
28 A: austenite B: bainite M: martensite P: pearlite The complete isothermal transformation diagram for an iron-carbon alloy of eutectoid composition.A: austeniteB: bainiteM: martensiteP: pearlite
29 Example ProblemUsing the isothermal transformation diagram for an iron-carbon alloy of eutectoid composition, specify the nature of the final microstructure of a small specimen that has been subjected to the following time- temperature treatments.The specimen begins at 760°C and that it has been held at this temperature long enough to have achieved a complete and homogeneous austenitic structure.(a) Rapidly cool to 250°C, hold for 100s, and quench to room temperature(b) Rapidly cool to 600°C, hold for 104 s, and quench to room temperature
30 Example Problem(a) Rapidly cool to 250°C, hold for 100s, and quench to room temperature(b) Rapidly cool to 600°C, hold for 104 s, and quench to room temperatureThe time-temperature-transformation diagram for an iron-carbon alloy of eutectoid composition and the isothermal heat treatments
31 Example Problem At 760°C: in the austenite region (g)— 100% austenite (a) Rapidly cool to 250°C, hold for 100s, and quench to room temperatureAt 760°C: in the austenite region (g)— 100% austeniteRapidly cool from 760°C to 250°C: 100% austeniteHold for 100 seconds at 250°C: 100% austeniteQuench to room temp.: 100% martensite
32 Example Problem At 760°C: in the austenite region (g)— 100% austenite (b) Rapidly cool to 600°C, hold for 104 s, and cool to room temperatureAt 760°C: in the austenite region (g)— 100% austeniteRapidly cool from 760°C to 600°C: 100% austeniteHold for 104 s at 250°C: 100% pearliteQuench to room temp.: 100% pearlite
33 Mechanical Behavior of Iron-Carbon Alloys PearliteCementite (Fe3C) is much harder but more brittle than ferrite (a).% Fe3C strength, ductilityMartensiteHardest and strongest, and most brittleVolume change crack formation during quenching
34 Mechanical Properties of Fe-C Systems • Fine Pearlite vs Martensite:• Hardness: fine pearlite << martensite.